Upload
vankhanh
View
218
Download
0
Embed Size (px)
Finite-size correction for first-principles point defect calculations using a supercell approach
Yu Kumagai1, and Fumiyasu Oba2,1
1Materials Research Center for Element Strategy, Tokyo Institute of Technology, Yokohama,
226-8503, Japan 2Department of Materials Science and Engineering, Kyoto University, Kyoto 606-8501, Japan
Point defects in semiconductors and insulators play a decisive role in determining materials properties. However, it is not straightforward to fully investigate their concentrations and atomic and electronic structures in experiments, and first-principles calculations have emerged as a valuable tool for the study of defects in recent years. First-principles calculations for solids usually adopt three-dimensional periodic boundary conditions. Then, charged defect calculations can include huge errors up to several eV due to the limitation of supercell sizes [1-3]. Recently, Freysoldt, Neugebauer, and Van de Walle (FNV) proposed a remarkable scheme to correct the finite size errors [3]. This allows us to estimate the correction energy up to the L-3 order, where L is the dimension of the supercell, without additional first-principles calculations. The great advantage is that it can be applied to computationally very demanding calculations using, for instance, hybrid functionals and quantum Monte Carlo, which can treat only very limited sizes of supercells. The original FNV correction scheme is, however, applicable only to cubic systems because it is assumed that the long-range Coulomb interaction is screened by a dielectric constant. Very recently, we extended the FNV correction scheme by rewriting the formalism using an anisotropic form with a dielectric matrix [4]. With systematic assessment of the corrective capability, the extended FNV scheme has been found to excellently correct the formation energies of a wide variety of charged defects in diverse materials. In this study, we apply the extended FNV scheme to the formation energy of the oxygen vacancy with q=+2 charge (VO
+2), Ef[VO+2], in lithium titanate β-Li2TiO3, which
has been studied for the use in lithium ion batteries. The crystal structure and removed oxygen ion are shown in Fig.1. As inferred from the layered structure, the diagonal components of the dielectric matrix are very different [4]. First-principles calculations were performed with the PAW method [5] as implemented in the VASP code [6], and calculation conditions were kept consistent with those in Ref. [4]. The correction energy of the FNV scheme is the sum of a point-charge (PC) correction energy and an alignmentlike term [4]. The latter is estimated from potential offset between the defect-induced potential (Vq/b) and PC potential (VPC,q), and can be written as –q∆VPC,q/b|far, where q is a defect charge, ∆VPC,q/b = Vq/b - VPC,q, and ∆VPC,q/b|far is ∆VPC,q/b far from a defect and its images [3, 4]. Figure 2(a) shows Vq/b, VPC,q, and ∆VPC,q/b of VO
+2 in a 2 × 2 × 2 supercell. Vq/b and VPC,q widely scatter even at the same distance from the defect, reflecting the anisotropic screening feature, and ∆VPC,q/b converges in a region far from the defect. ∆VPC,q/b|far was determined by averaging ∆VPC,q/b at the atomic positions outside of the sphere in contact with the Wigner-Seiz cell. Figure 2(b) shows Ef[VO
+2] without and with corrections at different levels as a function of cell size and shape. Without corrections, Ef[VO
+2] widely scatters depending on the supercell size and
FIG. 1. Crystal structure of β-Li2TiO3. The position of the oxygen vacancy introduced in this study is shown in circles.
FIG. 2. (a) Defect-induced potential (Vq/b), point-charge potential (VPC,q), and their differences (∆VPC,q/b) at the atomic sites in a β-Li2TiO3 2 × 2 × 2 supercell with VO
+2. The region for averaging ∆VPC,q/b and its averaged value are expressed in the width and height of the arrow, respectively. (b) Uncorrected and corrected formation energies of VO
+2 as a function of the supercell size and shape. Zero is set to the anisotropic FNV corrected formation energy calculated with the 2 × 3 × 1 supercell.
shape. The isotropic FNV correction with a dielectric constant, which is typically adopted by many authors, does not avail to correct Ef[VO
+2]. On the other hand, the anisotropic PC drastically reduces the cell size/shape dependence. The potential alignmentlike term in the anisotropic FNV scheme successfully corrects the remaining cell size/shape dependence, and it almost vanishes in large supercells. This work was supported by the MEXT Elements Strategy Initiative to Form Core Research Center “Tokodai Institute for Element Strategy (TIES)” and a Grant-in-Aid for Scientific Research on Innovative Areas "Nano Informatics" (grant number 25106005) from JSPS. References [1] S. Lany and A. Zunger, Phys. Rev. B 78, 235104 (2008). [2] H.-P. Komsa et al., Phys. Rev. B 86, 045112 (2012). [3] C. Freysoldt et al., Phys. Rev. Lett. 102, 016402 (2009). [4] Y. Kumagai and F. Oba, arXiv:1402.1226 (2014). [5] P. E. Blöchl, Phys. Rev. B 50, 17953 (1994). [6] G. Kresse and J. Hafner, Phys. Rev. B 47, 558 (1993).